doi:10.4236/jemaa.2010.211083 Published Online November 2010 (http://www.scirp.org/journal/jemaa)

**New Interfacial Shear-Horizontal Waves in **

**Piezoelectric Cubic Crystals **

**A.A. Zakharenko **

International Institute of Zakharenko Waves, Krasnoyarsk, Russia. E-mail: aazaaz@inbox.ru

Received September 15th_{, 2010; revised October 20}th_{, 2010; accepted October 23}rd_{, 2010. }

**ABSTRACT **

*This theoretical study reports results on acoustic wave propagation along the interface of two half-spaces representing *
*cubic crystals of both piezoelectric classes *43*m and *23 *with strong piezoelectric effect. In similar configurations, the *
*interfacial Maerfeld-Tournois waves can propagate along the interface of two transversely-isotropic materials of class *

6* mm, in which the shear-horizontal surface acoustic waves *(*SH-SAWs*)* called the Bleustein-Gulyaev *(*BG*)* waves can *
*also exist. Cubic piezoelectrics cannot support existence of the surface BG-waves, according to the recent report by *
*Gulyaev and Hickernell. Hence, new interfacial SH-waves are studied in this paper concerning unique direction *[101]

*of wave propagation in cubic crystals using different electrical boundary conditions *(*EBCs*)* of both metallized and *
*non-metallized interfaces. The new interfacial SH-waves can always propagate along the interface of two identical *
*piezoelectric crystals with opposite polarization. In this case, the calculated velocities for both EBCs coincide with the *
*velocity of the ultrasonic surface Zakharenko wave *(*USZW*)* propagating in direction *[101]* on the metallized surface of *
*a cubic piezoelectrics. It was also found that the new interfacial SH-waves can exist when wave propagation is along *
*the interface of two dissimilar half-spaces, for instance, the piezoelectric cubic crystals Bi*12*SiO*20* and Bi*12*GeO*20*. *

*Several calculations are also carried out as examples. PACS***:** 51.40.*+p, *62.65*.+k, *68.35*.Gy, *68.35*.Iv, *68.60.*Bs, *

74.25*.Ld. *

**Keywords****:*** New Shear-Horizontal Interfacial Wave, Strong Piezoelectric Effect, Piezoelectric Cubic Crystals, Solutions *
*for “Latent” Waves *

**1. Introduction **

The theoretical investigations carried out in 1971 by
Maerfeld and Tournois [1] introduced an acoustic
shear-horizontal (SH) wave guided by the common
inter-face of two semi-infinite media, if at least one of the
me-dia is a piezoelectric material. Maerfeld and Tournois
have stated the existence conditions for such waves
called the interfacial Maerfeld-Tournois (MT) waves,
which can also propagate along the interface of two
iden-tical transversely-isotropic crystals of class 6 mm, when
the *C*-axes of the crystals are in opposite directions,
sat-isfying the perpendicularity condition of the wave
propagation direction to an even-order symmetry axis.
This is similar to the other shear-horizontal surface
acoustic waves (SH-SAWs) simultaneously discovered
by Bleustein [2] and by Gulyaev [3] in the late 1960s,
which possess a hybridization between the mechanical
displacement *U*2 and electrical potential *φ* = *U*4. These

two types of SH-waves, namely the interfacial MT-waves and surface Bleustein-Gulyaev (BG) waves, can only propagate along surfaces of suitable crystal cuts of trans-versely-isotropic crystals of the hexagonal and tetragonal classes 6 mm and 4 mm. It is thought that these surface SH-waves have deeper penetration length and lower en-ergy loss than do surface Rayleigh waves [4]. Therefore, they can be easily excited and detected.

between two dissimilar piezoelectric crystals.

The purpose of this report is to introduce theoretical investigations of new interfacial SH-waves in piezoelec-tric cubic crystals with the strong piezoelecpiezoelec-tric effect. The Chalcogenide family crystals (Tl3VS4 and Tl3TaSe4 [7]) belonging to the cubic class 43m and possessing both zero temperature coefficients and strong piezoelec-tric coupling, are examined. In spite of their very large potential interest, especially for moderate frequency and large bandwidth, such ternary thallium Chalcogenides Tl3TaSe4 are not commercially available, probably due to their mechanical softness and fabrication difficulties. However, the piezoelectric ceramics of the point group symmetry 23 (Bi12SiO20 and Bi12GeO20 [8] and Bi12TiO20 [9]) can be used in piezoelectronics. Recently, new SH-SAWs [10] called the ultrasonic surface Zakharenko waves (USZWs) were discovered in such cubic piezo-electrics with the strong piezoelectric effect. Note that some piezoelectrics display colossal enhancement of piezoelectricity [11]. It is noted that over several hundred piezoelectric materials, particularly piezoelectric ceram-ics or composites, are known, for example see Ref. [12], having their intrinsic electromechanical coupling behav-iors. They are widely used today for different applica-tions such as filters and sensors, as well as actuators and ultrasonic generators.

Concerning fabrication of a structure consisting of two dissimilar crystals, a process called wafer bonding is utilized in the semiconductor industry, allowing two dif-ferent materials to be rigidly and permanently bonded along a plane interface, thus producing a composite bi-material [13]. It is noted that several hundred wafer bonding patents are annually deposited [14]. In addition, a similar second process called fusion bonding is used by the polymer industry to bring together two parts of dif-ferent solid polymers, thus enabling the manufacture of a heterogeneous bi-material with specific properties [15,16]. In the first process, wafers of two different crys-tals are stuck together through Van der Waals forces, after their surface has been mirror-polished. In the second, however, a fusion process followed by a cooling and consolidating period takes place at the interface. It is ob-vious that it is important to be able to inspect the strength of the bonding, possibly through non-destructive ultra-sonic evaluation. However, very few simple numerical investigations exist to compute the speed, etc., of interfa-cial waves when they exist.

**2. Theory **

**Figure 1** introduces a rectangular coordinate system (*x*1,

*x*2, *x*3) so that the *x*1*Ox*3 sagittal plane is perpendicular to
the even-order symmetry axis of a piezoelectric cubic
crystal and the *x*1-axis demonstrates wave propagation in

Monocrystal I
**x****1[101]**

**x****3**

**x****2**

0

Interface

Monocrystal II

**Figure 1. The rectangular coordinate system with the **
**x****2-axis directed along the interface of two half-spaces **

**where the ****x****1-axis is directed perpendicular to the **

**fig-ure plane. **

direction [101]. It is necessary to write governing equa-tions of linear piezoelasticity. Constitutive relaequa-tions are written as follows:

*E*

*ij* *ijkl kl* *ijm* *m*

*T* *C S* *e E* (1)

*m* *mij ij* *mn* *n*

*D* *e S* *g E* (2)

in which *Tij* and *Sij* are the stress and strain tensors,

re-spectively; *Dm* and *Em* are components of the electrical

displacement and electrical field (*Em* = – ∂*φ*/∂*xm* where *φ*

is the electrical potential); the indices *i*, *j*, *k*, *l* , *m*, and *n*

run from 1 to 3. According to the Voigt notation,* Cijkl*, *eijm*,

and *gmn* can be written as 6 × 6, 3 × 6, and 3 × 3 matrices

standing for the elasticity, piezoelectricity, and dielectricity
tensors, respectively. It is assumed that studied materials
are free of body forces and inertial effects as well as body
electric charge. The equilibrium equations are as follows:
∂*Tij*/∂*xj* = 0 and ∂*Di*/∂*xi* = 0.

The equation of motion of an elastic medium is written as follows:

2 2

*ik* *i*
*k*

*T*

*x* *t*

*U*

(3)

where *ρ* and *Ui* denote the mass density and mechanical

displacement components; *t* is time. Using equations
from (1) to (3), the coupled equations of motion for a
piezoelectric medium are written in the following forms:

2 2 2

4

2

2 2

4 _{0}

*l* *i*

*ijkl* *kij*

*j* *k* *j* *k*

*k*

*ijk* *ij*

*i* *j* *i* *j*

*U* *U* *U*

*C* *e*

*x x* *x x* *t*

*U* *U*

*e* *g*

*x x* *x x*

_{} _{}

(4)

###

###

0

1 1 2 2 3 3

exp

*i* *i*

*U* *U* _{}*jk n x* *n x* *n x* *j t* _{}

where the index *i* runs from 1 to 4; *Ui*0 is an initial

am-plitude. The imaginary unity is defined as j = (–1)1/2_{ and }

*ω* is the angular frequency. *k* is the wavenumber in the

*k*-space with the following components {*k*1, *k*2, *k*3} = *k*{*n*1,

*n*2, *n*3} and {*n*1, *n*2, *n*3} are the directional cosines. {*x*1, *x*2,

*x*3} are the components of real space.

Leaving only equations for waves with polarization perpendicular to the sagittal plane and non-zero compo-nents of the material tensors, the coupled equations of motion in Equation (4) can then be written in the follow-ing convenient forms:

2 2 2 2 2

2 2 4 4

44 2 2 16 2 34 2

1 3 1 3

*U* *U* *U* *U* *U*

*C* *e* *e* 2

2

*x* *x* *x* *x*

*t*

2 2 2 2

2 2 4 4

16 2 34 2 11 2 2

1 3 1 3

0

*U* *U* *U* *U*

*e* *e* *g*

*x* *x* *x* *x*

_{} _{} _{}
_{} _{}
(5)

where the mechanical displacement component *U*2 is
di-rected along the *x*2-axis shown in **Figure 1**:

###

###

0

2,4 2,4exp 1 1 3 3 *ph*

*U* *U* _{}*jk n x* *n x* *V t* _{} (6)

In Equation (6), the phase velocity is defined as *vph* =

/*k*. Equation (5) describes wave propagation in direction
[101] with *e*14 = *e*36 = 0 and the non-zero piezoelectric
constants {*e*16, *e*34}. It is thought that such cuts of cubic
crystals can be readily done. Note that all propagation
directions perpendicular to direction [010] can exist
giv-ing *C*44 = *C*66 and *g*11 = *g*33 concerning piezoelectric cubic
crystals.

Using Equations (5) and (6), the tensor form of equa-tions of motion can be written with corresponding GL-components in the Green-Christoffel equations:

, and

where *n*3 = *k*3/*k*. Therefore, the
fol-lowing system of two homogeneous equations must be
resolved:

###

2###

22 44 1 3

*GL* *C* *n*

###

244 11 1 3

*GL* *g* *n*

2

24 42 16 34 34 3

*GL* *GL* *e* *e* *e n*

###

###

###

2_{0}

2

22 44 4 24

0 4

42 44

0 0

*ph* *t* *U*

*GL* *C* *V* *V* *GL*

*U*
*GL* *GL*
_{} _{} _{}
_{} _{} _{ }
_{ }
(7)

The directional cosines in Equation (7) are defined as
follows: *n*1≡ 1, *n*2≡ 0 and *n*3 = *n*3. Setting the
determi-nant of the coefficient matrix in Equation (7) equal to
zero, several characteristics can be found such as a
suit-able phase velocity *Vph* satisfying boundary conditions

discussed in the following section and four polynomial
roots *n*3(*p*)(*Vph*), as well as the functions *U*20(*Vph*) and

*U*40(*Vph*). It is thought that it is convenient to utilize the

functions *U*20(*Vph*) and *U*40(*Vph*) in the following forms:

and .

0 4

*U* *GL*_{42} _{4}

Using the piezoelectric constants 16 34 for direc-tion [101], the following polynomial can be introduced from Equation (7):

0

2 4

*U* *GL*

*e* *e*

###

2###

2 23 3

1*K m _{e}*

*Bm*4

*K*0 with 2

_{e}4
4
*ph*
*e*
*t*
*V*
*B* *K*
*V*

(8)

where *m*3 = 1 + *n*32. In Equation (8), *Ke*2 is the static

coef-ficient of the electromechanical coupling (CEMC):

###

###

2 2

16 44 11

*e*

*K* *e* *C g* . Note that the speed *VSH* of the bulk

SH-wave reads:

###

_{2}

###

1 2 4 1*SH* *t* *e*

*V* *V* *K* (9)

It is obvious that Equation (8) has two roots:

###

###

###

###

2 2 1,2 3_{2}16 1 2 1

*e*

*e*

*e*

*B* *B* *K* *K*

*m*
*K*
2
(10)

Hence, four polynomial roots (eigenvalues) of Equation (7) are as follows:

1,2,3,4 1,2

3 1

*n* *m*_{3} (11)

It is noted that the eigenvector {*U*20, *U*40} in Equation (7)
can be obtained for each eigenvalue *n*3.

Note that all complex roots can be calculated when the
expression *B*2_{ – 16}_{K}

*e*2(1 + *Ke*2) under square root in

Equation (10) is negative. This fulfills for *Vph* < *VK*

ob-tained from the following equation *B*2_{ – 16}_{K}

*e*2(1 + *Ke*2) =

0 and defined by the following formula:

4

*K* *K t*

*V* *V* with _{2} _{1} 2 2

*K* *Ke* *Ke* *Ke*

(12)

It is clearly seen that both the factor *αK* in Equation (12)

and the function *f*(*Ke*2) = (1 + *Ke*2)1/2 in Equation (9) are

functions of the CEMC *Ke*2. Discussions about behavior

of polynomial roots and the function *αk* can be found in

Ref. [10]. However, it is necessary to briefly discuss that
only complex polynomial roots can exist for *Vph* < *VK* and

that for *Ke*2 < *K*02 (*K*02 = 1/3) there are all imaginary roots
for *Vph* > *VK*, but a very large* Ke*2 > *K*02 gives real roots
for *Vph* > *VK*. It is noted that only complex/imaginary

roots with negative/positive imaginary parts for medium
I/II in **Figure 1 **are chosen in order to have wave

damp-ing towards the each half-space depth from the common
interface. Probably, surface waves cannot be found in the
cubic crystals with a large *Ke*2 > 1/3 in the *Vph*-range: *VK*

< *Vph* < *VSH*. It is thought that a large *Ke*2 can be observed

accord-ing to the recent results obtained in Ref. [11]. І І І І І І І І

32 44 3 2 34 3 4

1,2

*p* *p* *p* *p*

*p*

*T* *F* *C k* *U* *e k* *U*

*p*

###

_{}

_{}

**3. Boundary Conditions for Interfacial **

**SH-Waves **

ІІ ІІ ІІ ІІ ІІ ІІ ІІ ІІ
32 44 3 2 34 3 4

1,2

*p* *p* *p* *p*

*p*

*T* *F* *C k* *U* *e k* *U*

*p*

###

_{}

_{}(14)

There is single boundary at *x*3 = 0 in **Figure 1**
represent-ing the interface between two half-spaces, at which
suit-able requirements can be chosen. These several
require-ments called boundary conditions must be satisfied for
propagation of the interfacial SH-waves, which must
damp from the common interface towards depth of each
half-space. Using the coordinate system in **Figure 1**, only

eigenvalues with negative imaginary parts must be
cho-sen for the medium with negative values of the *x*3-axis.
Also, only eigenvalues with positive imaginary parts
must be chosen for the medium with *x*3 > 0. There are
two mechanical boundary condition such as equality of
the mechanical displacements *U*2 (*U*2I = *U*2II) where

Note that the superscripts “I” and “II” are for the first and
second media, respectively. There are two electrical
boundary conditions at *x*3 = 0: continuity of the normal
component *D*3 of the electrical displacements, where

І І І І І

І І І

32 34 3 2 33 3 4

1,2

*p* *p* *p* *p*

*p*

*D* *F* *e k* *U* *g k* *U*

*p*

###

_{}

_{}

ІІ ІІ ІІ ІІ ІІ

ІІ ІІ ІІ

32 34 3 2 33 3 4

1,2

*p* *p* *p* *p*

*p*

*D* *F* *e k* *U* *g k* *U*

*p*

###

_{}

_{}(15)

and continuity of the electrical potential *U*4 = ( I = II)
where

I I( )

1,2
I( )
*p* *p*
*p*
*F*

###

and II II( ) II( )1,2
*p* *p*
*p*
*F*

###

І І І 2 2 1,2*p*

*p*

*p*

*U* *F* *U*

###

and ІІ ІІ ІІ 2

1,2 2

*p* *p*

*p*

*U* *F* *U*

###

(13)and equality of the normal components of the stress
ten-sor, *T*I

32 = *T*II32, where

###

*t*

_{}2 (16)

Therefore, the boundary-condition determinant (BCD4) of fourth-order for the interfacial waves can be written using the following four homogeneous equations:

I(1) I(2) II(1) II(2)

2 2 2 2

I I(1) I(1) I I(2) I(2) II II(1) II(1) II II(2) II(2)

44 3 2 44 3 2 44 3 2 44 3 2

I I(1) I(1) I I(2) I(2) II II(1) II(1) II II(2) II(2)

34 3 4 34 3 4 34 3 4 34 3 4

I(1) I(2) II(1) II(

4 4 4 4

*U* *U* *U* *U*

*C k U* *C k U* *C k* *U* *C k* *U*

*e k U* *e k* *U* *e k* *U* *e k* *U*

*U* *U* *U* *U*

(1) (2) 2) (3) (4) I I(1) I(1) I I(2) I(2) II II(1) II(1) II II(2) II(2)

34 3 2 34 3 2 34 3 2 34 3 2

I I(1) I(1) I I(2) I(2) II II(1) II(1) II II(2) II(2)

33 3 4 33 3 4 33 3 4 33 3 4

*F*
*F*
*F*
*F*

*e k U* *e k U* *e k* *U* *e k* *U*

*g k U* *g k U* *g k* *U* *g k* *U*

_{} _{}
0
0
0
0
(17)

Using the mechanical and electrical boundary conditions at

*x*3 = 0 such as *U*2I = *U*2II, *σ*32I = *σ*32II, I = 0 and II = 0, the

BCD4 of the coefficient matrix for the case of metallized interface can be obtained from the following equations:

I(1) I(2) II(1) II(2)

2 2 2 2

I I(1) I(1) I I(2) I(2) II II(1) II(1) II II(2) II(2)

44 3 2 44 3 2 44 3 2 44 3 2

I I(1) I(1) I I(2) I(2) II II(1) II(1) II II(2) II(2)

34 3 4 34 3 4 34 3 4 34 3 4

I(1) I(2) 4 4 II(1) I 4 4 0 0 0 0

*U* *U* *U* *U*

*C k U* *C k U* *C k* *U* *C k* *U*

*e k U* *e k* *U* *e k* *U* *e k* *U*

*U* *U*

*U* *U*

_{(2)}(1)

(3)
(4)
I(2)
0
0
0
0
*F*
*F*
*F*
*F*
_{}
_{} _{}
(18)

The complete mechanical displacement *U*2Σ and
elec-trical potential *φ*Σ_{ = }_{U}

4Σ are written for each half-space as follows:

0

###

2,4 2.4 1 1 3 3

1,2

exp

*p* *p* *p*

*ph*
*p*

*U* *F U* *jk n x* *n x* *V*

###

_{} (19)

The corresponding weight functions *F*(*p*)_{ are found }
from Equations (17) and (18), which can give the same
eigenvectors (*U*20(1), *U*40(1)) and (*U*20(2), *U*40(2)) for two
equal eigenvalues *n*3(1) = *n*3(2) in each half-space and

hence 1

*F* *F*

1 2 . It is obvious that the weight factors

*F* *F* will zero the complete mechanical

dis-placement *U*2Σ and electrical potential *φ*Σ in Equations (17)

and (18). That can mean that they are “latent”
character-istics. On the other hand, eigenvalues *n*3(1) ≠ *n*3(2) give
corresponding eigenvectors (*U*20(1), *U*40(1)) and (*U*20(2),

*U*40(2)) as well as *F* 1 *F* 2 resulting in non-zero
dis-placements, which must be equal at the interface damping
towards the depth of both media.

**4. Results and Discussions **

suitable cuts of the transversely-isotropic materials, in
which the surface BG-waves can also exist. Note that the
velocity of interfacial Maerfeld-Tournois (MT) wave in
similar materials with opposite polarization coincides
with the velocity *VBGm* of the surface BG-wave

propagat-ing along the metallized surface of transversely-isotropic
piezoelectrics, *VBGm* = *VSH*[1 – (*Ke*2/(1 + *Ke*2))2]1/2 [2]. This

can mean that some similarity occurs between the
inter-facial MT-waves and surface BG-waves when the
trans-versely-isotropic materials are treated. The velocity *VBG*

of the BG-wave with the non-metallized surface is
calcu-lated with the following formula: *VBG* =* VSH*{1 – (*Ke*2/[(1

+ *Ke*2)(1 + *g*11/*g*0)])2}1/2. Due to the fact that the surface
Bg-waves and the interfacial MT-waves cannot exist in
piezoelectric cubic crystals, the existence of new surface
SH-waves called the ultrasonic surface Zakharenko
waves (USZWs) was studied in the cubic crystals (see
Ref. [10]) and the new interfacial SH-wave existence is
studied in this paper.

The material constants and USZW characteristics for
several cubic crystals with strong piezoelectric effect are
listed in **Tables 1** and **Table2**, respectively. It was found

that the velocities of the new interfacial waves with
met-allized interface are coincide with the *VBGm*. This is also

true for the velocities of the interfacial MT-waves and the USZWs on the metallized surface. That illuminates common wave speed characteristics among the different

waves. Therefore, they can be calculated with the for
mula for *VBGm* written above. It is noted that all the above

mentioned velocities were calculated using different
boundary-condition determinants. However, it was found
that the velocity of the USZWs on the non-metallized
surface cannot be calculated with the formula for *VBG*.

For instance, the formula for *VBG* gives the value of *V*1 ~
848.6 m/s instead of the **Table 2** value of *Vnew* ~ 848.1

m/s for Tl3TaSe4. The velocity *V*1 is significantly closer
to the velocity *vSH* of bulk waves (see **Table 2**) than the

true velocity* Vnew* obtained numerically. Therefore, it is

obvious that the penetration depth of the USZWs in
pie-zoelectric cubic crystals will be smaller than that for the
surface BG-waves in the transversely-isotropic
monocrystals. This is an advantage of the USZWs. Note
that all the wave characteristics were calculated with an
accuracy of about 1 μm/s. This is useful and allows the
distinguishing of *Vph*-solutions when they are close to

each other.

**Figure 2** shows the phase velocity solutions for the new

interfacial waves (*Vin*) in the Chalcogenides Tl3TaSe4 and
Tl3VS4 pertaining to class 43m, *Vin* = *Vnew,m*, using

simi-lar materials for the acoustic systems with opposite
po-larization and both the metallized and non-metallized
interfaces, *Vin* = *Vin,m*. The finding of *Vin* for the cubic

crystals Bi12SiO20 and Bi12GeO20 of class 23 is shown in

**Figure 3** using the same configuration consisting of

**Table 1. The material constants: the material density ****ρ****, non-zero elastic ****C****44, piezoelectric ****e****14 and dielectric ****g****11 constants for the **
**SH-wave propagation in the piezoelectric cubic crystals [7,8,9] with the strong piezoelectric effect. Note that the dielectric **
**con-stant of a vacuum is ****g****0 = 0.08854 [10–10 F/m]; ****e****16[101] = – ****e****14[100] and**** e****34[101] = ****e****14[100]. The coefficient of electromechanical coupling **
**(CEMC)**** K****e****2 in the last column was calculated with the following formula: ****K****e****2 = ****e****142/(****C****44****g****11). **

Material Density, *ρ* [kg/m3_{] } _{C}

44, 1010 [N/m2] *e*14[100] [C/m2] *g*11/*g*0 *Ke*2

Tl3TaSe4 (43 m) 7280 0.410 0.320 10.1 0.2793

Tl3VS4 (43 m) 6140 0.470 0.550 34.8 0.2089

Bi12TiO20 (23) 11200 2.600 1.100 47.0 0.1118

Bi12SiO20 (23) 9070 2.451 1.122 41.1 0.1412

Bi12GaO20 (23) 9300 2.600 1.100 145.7 0.0361

Bi12GeO20 (23) 9200 2.562 0.983 37.7 0.1131

**Table 2. The wave characteristics: the velocities ****V****K****, ****V****t****4, and ****V****SH**** (all in m/s) as well as the velocities ****V****new**** and ****V****new,m**** of the **
**new-SH-SAWs (USZWs) on the free and metallized surfaces, respectively, for the piezoelectric cubic crystals with the strong **
**piezoelectric effect when the wave propagation is along direction [101]. The last column lists the non-dimensional values of **

**the CEMC ****K****2 calculated with formula (20). Note that one can calculate that ****V****BG****(Bi12SiO20) = 1756.096654 m/s is larger than **

**V****new****(Bi12SiO20) and the same occurs for ****V****BG****(Bi12GeO20) = 1760.569112 m/s. **

Material *VK * *Vt*4 *VSH * *Vnew * *Vnew,m * *K*2

Tl3TaSe4 (43m) 846.9869546 750.4577358 848.8104580 848.125556 828.335498 0.047

Tl3VS4 (43m) 948.1841318 874.9127458 961.9607843 961.927246 947.491302 0.030

Bi12TiO20 (23) 1495.282953 1523.62350 1606.562692 1606.556882 1598.414906 0.010

Bi12SiO20(23) 1677.148081 1643.872053 1756.104245 1756.089613 1742.609095 0.015

Bi12GaO20(23) 1326.112526 1672.034367 1701.927576 1701.927574 1700.895518 0.001

-0.05 0 0.05

820 850Phase velocity, m/s

BCD

4

Im(mBCD4)

Re(BCD4)

*VK*
*Vin*

(a)

Phase velocity, m/s

BCD

4

-0.05 0 0.05

945 950 Re(BCD4)

Im(mBCD4)

*VK*

*Vin*

(b)

**Figure 2. The dependence of the boundary-condition **

**deter-minants (BCD4) on the phase velocity ****V****ph**** for direction [101] **

**of the new interfacial wave (****V****in****) propagation in the systems **

**Tl3TaSe4 (a) and Tl3VS4 (b) with opposite polarization using **
**the interface metallization (mBCD4) and non-metallized **
**interface (BCD4). **

Phase velocity, m/s

BCD

4

-100 0 100

1740 1760

Re(BCD4) Im(mBCD4)

*Vin(Bi*12SiO20)

*Vin(Bi*12GeO20)

**Figure 3. The dependence of the boundary-condition **

**deter-minants (BCD4) on the phase velocity ****V****ph**** for direction [101] **

**of the new interfacial wave (****V****in****) propagation in the systems **

**Bi12SiO20 and Bi12GeO20 with opposite polarization using the **
**interface metallization (mBCD4) and non-metallized **
**inter-face (BCD4). **

similar materials. It was thought that the crystals Bi12SiO20 and Bi12GeO20 can be used together to support propagation of the new interfacial waves in dissimilar

material, because their bulk SH velocities *vSH* are

rela-tively close to each other and also true for *Vin*. The BCD4

behaviors for the dissimilar materials are shown in

**Figure 4**, in which it is clearly seen that there are

solu-tions for the Bi12SiO20/Bi12GeO20 configuration. Using
the normal polarization for the crystals Bi12SiO20 and
Bi12GeO20, only the velocity *Vin,m* for the metallized

in-terface was found having the value of *Vi n , m* =

1746.926119 m/s. The *Vin,m* value is larger than the value

of *Vnew,m* for Bi12SiO20 listed in **Table 2** and smaller than
the value of *Vnew,m* for Bi12GeO20. However, the
configu-ration with the opposite-polarized crystals Bi12SiO20 and
Bi12GeO20 demonstrates existence of both velocities *Vin,m*

and *Vin* for the metallized and non-metallized interfaces,

*Vin,m* = 1746.926119 m/s and *Vin* = 1747.138149 m/s. It is

clearly seen that the values of *Vin,m* and *Vin* are close to

each other but distinguishable in the calculations.
In the case of known values of the *Vin,m* and *Vin*, the

ex-istence of the new interfacial waves for both the electrical
boundary conditions allows evaluation of the coefficient
of electromechanical coupling (*K*2_{): }

,

2 _{2} *in* *in m*

*in*

*V* *V*

*K*

*V*

(20)

The value of *K*2_{ calculated with formula (20) is very }
small for the crystals with the strong piezoelectric effect
(see the tables) and is equal to *K*2_{ ~ 0.000243. This is }
only ~ 0.0243% and significantly smaller than ~ 1% for
Bi12GeO20 listed in **Table 2**. It is also noted that the
in-terfacial wave propagation can be studied in suitable
two-layer structures consisting of various cubic
piezo-magnetics [17,18]. Note that a study of interfacial wave
propagation in non-cubic piezomagnetics was recently
introduced in Ref. [19].

BCD

4

Phase velocity, m/s -80

-40 0 40

1740 1745 1750 1755

*Vin,m*

Re(BCD4) Im(mBCD4)

**Figure 4. The dependence of the boundary-condition **

**deter-minants (BCD4) on the phase velocity ****V****ph**** for direction [101] **

**of the new interfacial wave (****V****in,m****) propagation in the **

**5. Conclusions **

This theoretical report was concerned with the interfacial wave propagation in cubic crystals with strong piezoelec-tric effect, in which the surface Bleustein-Gulyaev waves cannot exist. This was recently mentioned in Ref. [5] by Gulyaev and Hickernell. It was illuminated that the new interfacial waves can always be found in acoustic systems consisting of two half-spaces representing identical mate-rials with opposite polarization. Also, the new interfacial waves can exist in dissimilar materials solidly coupled at their interface, for instance, in the Bi12SiO20/Bi12GeO20 sys-tem, using the electrical boundary conditions of both the metallized and non-metallized interfaces. Note that the theoretically obtained results can be useful to design ex-periments for measuring interfacial properties by the mi-crowave technologies.

### 6

**. Acknowledgements **

The author is grateful to the Referees for useful notes.

**REFERENCES **

[1] C. Maerfeld and P. Tournois, “Pure Shear Elastic Surface
Wave Guide by the Interface of Two Semi-Infinite
Me-dia,” *Applied Physics Letters,* Vol. 19, No. 4, 1971, pp.
117-118.

[2] J. L. Bleustein, “A New Surface Wave in Piezoelectric
Materials,” *Applied Physics Letters,* Vol. 13, No.12, 1968,
pp.412-413.

[3] Yu. V. Gulyaev, “Electroacoustic Surface Waves in
Sol-ids,” *Soviet Physics Journal of Experimental and *
*Theo-retical Physics Letters,* Vol. 9, No.1, 1969, pp. 37-38.
[4] G. A. Maugin, “Elastic Surface Waves with Transverse

Horizontal Polarization,” *Advances in Applied Mechanics*,
Vol. 23, 1983, pp. 373-434.

[5] Yu. V. Gulyaev and F. S. Hickernell, “Acoustoelectronics: History, Present State, and New Ideas for a New Era,”

*Acoustical Physics Reports*, Vol.51, No.1, 2005, pp.
101-110.

[6] G. G. Kessenikh and L. A. Shuvalov, “Transverse Surface Waves in Piezoelectric Crystals of Classes 622 and 422,”

*Ferroelectrics,* Vol. 42, No. 1, 1982, pp. 149-152.
[7] J. Henaff, M. Feldmann and M. A. Kirov, “Piezoelectric

Crystals for Surface Acoustic Waves (Quartz, LiNbO3,

LiTaO3, Tl3VS4, Tl3TaSe4, AlPO4, GaAs),” *Ferroelectrics,*

Vol.42, No.1, 1982, pp. 161-185.

[8] A. A. Zakharenko, “Love Type Waves in Layered Sys-tems Consisting of Two Piezoelectric Cubic Crystals,”

*Journal of Sound and Vibration*, Vol. 285, No. 4-5, 2005,
pp. 877-886.

[9] V. P. Kamenov, Y. Hu, E. Shamonina, K. H. Ringhofer and V. Ya. Gayvoronsky, “Two-Wave Mixing in (111)-Cut Bi12SiO20 and Bi12TiO20 Crystals:

Characteriza-tion and Comparison with the General OrientaCharacteriza-tion,”

*Physical Review E,* Vol. 62, No. 2, 2000, pp. 2863-2870.
[10] A. A. Zakharenko, “New Solutions of Shear Waves in

Piezoelectric Cubic Crystals,” *Journal of Zhejiang *
*Uni-versity SCIENCE A,* Vol. 8, No. 4, 2007, pp. 669-674.
[11] Zh. Wu and R. E. Cohen, “Pressure-Induced Anomalous

Phase Transitions and Colossal Enhancement of
Piezo-electricity in PbTiO3,” *Physical Review Letters,* Vol. 95,

No. 3, 2005, p. 4.

[12] R. C. Pohanka and P. L. Smith, “Recent Advances in Piezoelectric Ceramics”, Marcel Dekker, New York, 1988.

[13] U. Gösele and Q. Y. Tong, “Semiconductor Wafer
Bond-ing,” *Annual Review of Material Science,* Vol. 28, 1998,
pp. 215-241.

[14] M. Alexe and U. Gösele, “Wafer Bonding,” Springer, Berlin, 2003.

[15] C. A. Harper, “Handbook of Plastics, Elastomers and Composites,” 3rd Edition, McGraw-Hill, New York, 1996.

[16] C. Ageorges and L. Ye, “Fusion Bonding of Polymer Composites,” Springer, Berlin, 2002.

[17] A. A. Zakharenko, “First Evidence of Surface SH-Wave
Propagation in Cubic Piezomagnetics,” *Journal of *
*Elec-tromagnetic Analysis and Applications,* Vol. 2, No. 5,
2010, pp. 287-296.

[18] Y. Huang, X.-F. Li and K. Y. Lee, “Interfacial Shear
Horizontal (SH) Waves Propagating in a Two-Phase
Pie-zoelectric/Piezomagnetic Structure with an Imperfect
In-terface,” *Philosophical Magazine Letters,* Vol. 89, No. 2,
2009, pp. 95-103.

[19] A. K. Soh and J. X. Liu, “Interfacial Shear Horizontal Waves in a Piezoelectric-Piezomagnetic Bi-Material,”